Spatially Precise Transfer of Patterned Monolayer WS2 and ...nano.eecs. AEM_2019_2D... the substrate...
Embed Size (px)
Transcript of Spatially Precise Transfer of Patterned Monolayer WS2 and ...nano.eecs. AEM_2019_2D... the substrate...
Spatially Precise Transfer of Patterned Monolayer WS2 and MoS2 with Features Larger than 104 μm2 Directly from Multilayer Sources Hannah M. Gramling,† Clarissa M. Towle,‡,∥ Sujay B. Desai,§,∥ Haoye Sun,‡ Evan C. Lewis,†
Vu D. Nguyen,† Joel W. Ager,‡,∥ Daryl Chrzan,‡,∥ Eric M. Yeatman,⊥ Ali Javey,§,∥
and Hayden Taylor*,†
†Department of Mechanical Engineering, ‡Department of Materials Science and Engineering, and §Department of Electrical Engineering and Computer Sciences, University of California, Berkeley, Berkeley, California 94720, United States ∥Materials Sciences Division, Lawrence Berkeley National Laboratory, 1 Cyclotron Road, Berkeley, California 94720, United States ⊥Department of Electrical and Electronic Engineering, Imperial College London, Exhibition Road, London SW7 2AZ, U.K.
*S Supporting Information
ABSTRACT: A current challenge in the processing of 2D materials, or “van der Waals (vdW) solids”, is the transfer of 2D layers from source crystals and growth substrates onto target substrates. Transferas opposed to direct growth and patterning on the targetenables low-temperature processing of the target as well as the use of diverse target materials. These two attributes will allow the assembly of vdW heterostructures to realize devices exploiting the unique properties of vdW materials. Until now, however, there has been no effective method for transferring regions of monolayer material of controlled shape from a multilayer source. We introduce such a method and demonstrate its use in the spatially controlled transfer of arrays of single-layer MoS2 and WS2 sheets from multilayer crystals onto SiO2 substrates. These sheets have lateral sizes exceeding 100 μm and are electronically continuous. The method offers a scalable route to parallel manufacturing of complex circuits and devices from vdW materials. KEYWORDS: nanomanufacturing, transfer, scalable, two-dimensional materials, MoS2, WS2, exfoliation
■ INTRODUCTION van der Waals (vdW) solids are composed of single- to few- atom-thick “two-dimensional” layers loosely bound to each other by van der Waals forces. Their thinness results in extreme mechanical flexibility and exceptional properties, enabling many applications1 including in electronics,2,3
photonics,4 and chemical sensing.5 A growing appreciation of the properties of 2D materials has enabled increasingly sophisticated material heterostructures6,7 and increasingly integrated circuits containing, to date, over 100 2D material- based devices.8 Interfaces between semiconducting, conduct- ing, and insulating 2D materials find applications in, for example, field-effect transistors (FETs),9 memristive memo- ries,10 diodes,11 including light-emitting diodes (LEDs),12,13
photodetectors,12 photovoltaics,14 and catalysis.14
However, to fabricate multimaterial 2D structures through sequential vapor-phase deposition, lithography, and etching steps on a single substrateas in conventional semiconductor manufacturingis fraught with difficulties. First, although single-layer vapor-phase deposition techniques such as chemical vapor deposition are now maturing,1,15 the develop- ment of processes to deposit one specific 2D material on top of
another, while possible,16,17 is time-consuming (e.g., 26 h required15 for uniform monolayer MoS2 or WS2 on SiO2). Moreover, continuous layers of uniform thickness may prove impractical to produce because of lattice mismatches or chemical incompatibilities. While some fabrication flows actually exploit selective deposition characteristics to form overlap junctions (
thermal budgets and preclude the use of polymeric substrates, which are highly desirable for flexible electronics and would truly take advantage of 2D materials’ inherent flexibility.9
Attention has therefore turned to transfer-based assembly methods. Techniques using the surface tension of liquids to maneuver 2D monolayers into position offer limited spatial precision, are prone to wrinkling and folding,20 and introduce residues at the monolayer−substrate interface.1 Dry transfer (exfoliation) techniques have harnessed normally applied,21
shearing,22 and mixed-mode23 mechanical stresses to separate material from naturally occurring and synthetic sources. Several of these methods provide some within-layer dimen- sional precision, but layer thickness selectivity when exfoliating from multilayer sources has often been limited (Supporting Information Figure S1). Yet atomic monolayers are generally essential, e.g., for achieving a direct bandgap in MoS2.
What is needed is a technique with precision in all three dimensions, that can handle continuous sheets with lateral dimensions of many tens of micrometers or larger. Such large lateral sheet dimensions are needed for at least two possible purposes: (1) to provide material on which can be created integrated circuits with many submicrometer devices in a predefined spatial arrangement or (2) to define the boundaries of, e.g., powerful individual visible light emitters or sensitive detectors requiring dimensions in the tens of micrometers or larger. Moreover, a process that simultaneously achieves shape selectivity and monolayer selectivity is desirable for forming arrays of heterostructures by enabling the deposition of a
patterned monolayer array at the final substrate (which may already have patterned monolayer arrays on its surface). Recently, the prospects for monolayer exfoliation to be used
as a manufacturing process have improved markedly with the discovery that a thin Au film can be used to mediate the single- step exfoliation of large-area monolayers (>104 μm2) from multilayer sources.26,27 What that work did not achieve was precise control of monolayer shape or position (Figure S1), meaning that one was still required to comb over a target substrate for usable material. Recent work leveraging the same principle has demonstrated the transfer of larger area sheets,28
though subsequent patterning of material deposited on the substrate is necessary to form devices. The principles underlying this monolayer selectivity have
recently started to be understood.29,30 Essentially, atomic-scale modeling30 shows that when a metal is evaporated onto a 2D material crystal, the lattice mismatch between the metal and the 2D material induces a compressive strain in the top layer of the 2D material, weakening the bond between the top and second 2D layers so that a crack preferentially propagates between them when a load is applied (see also Supporting Information section S2). This crucial phenomenon removes the need for atomically precise etching of 2D materials prior to exfoliation of defined shapes of material. It therefore points toward the development of exfoliation-based transfer of patterned vdW monolayer materials. The manufacturing process that we introduce (Figure 1)
uses gold-mediated exfoliation in conjunction with a litho-
Figure 1. Process for producing patterned monolayers. The process for patterning and transferring van der Waals monolayers uses standard photolithography techniques. It relies on the use of a thick handle layer (here, photoresist, step 2) to pattern the gold and the underlying layered bulk material as well as to offset the adhesive transfer medium from the bulk, thus permitting transfer of only the patterned regions.
ACS Applied Electronic Materials Article
DOI: 10.1021/acsaelm.8b00128 ACS Appl. Electron. Mater. 2019, 1, 407−416
http://pubs.acs.org/doi/suppl/10.1021/acsaelm.8b00128/suppl_file/el8b00128_si_001.pdf http://pubs.acs.org/doi/suppl/10.1021/acsaelm.8b00128/suppl_file/el8b00128_si_001.pdf http://pubs.acs.org/doi/suppl/10.1021/acsaelm.8b00128/suppl_file/el8b00128_si_001.pdf http://pubs.acs.org/doi/suppl/10.1021/acsaelm.8b00128/suppl_file/el8b00128_si_001.pdf http://pubs.acs.org/doi/suppl/10.1021/acsaelm.8b00128/suppl_file/el8b00128_si_001.pdf http://dx.doi.org/10.1021/acsaelm.8b00128
graphically patterned handle layer to transfer arrays of monolayer regions with controlled shape, size, and separation. Our approach delivers a far higher areal density of usable, continuous monolayer material than unpatterned exfolia- tion26,27,29 and does so in predictable relative locations so that arrays of devices can subsequently be created in a systematic way.
■ METHODS Overview and Novelty. The process for creating patterned
monolayers is shown in Figure 1. It makes use of the recently established gold-mediated monolayer-selective exfoliation phenomen- on but adds a pre-exfoliation patterning stage in which photo- lithography followed by etching (wet etching of the gold, then plasma etching of the 2D material) defines the edges of regions to be exfoliated. What is particularly new and advantageous about this process is that the etching process does not need to be atomically precise: rather, the plasma etch creates crack initiation locations at the edges of the desired regions of material, while the deposition of the metal film ensures that those cracks propagate between the first and second layers of the 2D material. What is also demonstrated for the first time is spatial predetermination of where these regions of material are exfoliated. Making blanket contact between a transfer adhesive and a gold-coated 2D crystalas in previous reportsdoes, every so often, produce some very large areas (>104 μm2) of monolayer material, but they are ultimately very sparse on the substrate and their locations cannot be predicted. Etching material on the substrate post-transfer would not overcome this limitation. Patterning the crystal before exfoliation, as we do, initiates cracks that succeed in dictating where ma